d 5706 - 97 _rdu3mdytotc
NOTICE:¬This¬standard¬has¬either¬been¬super NOTICE:¬Thi s¬standard¬has¬either¬been¬superceded¬and¬replaced¬by¬a¬new¬versio ceded¬and¬replaced¬by¬a¬new¬version¬or¬discontinued.¬ n¬or¬discontinued.¬ Contact¬ASTM¬International¬(www.as Contact¬ASTM¬Inter national¬(www.astm.org)¬for¬the¬lates tm.org)¬for¬the¬latest¬information.¬ t¬information.¬
Designation: D 5706 – 97
An American National Standard AMERICAN SOCIETY FOR TESTING AND MATERIALS 100 Barr Harbor Dr., West Conshohocken, PA 19428 Reprinted from the Annual Book of ASTM Standards. Copyright ASTM
Standard Test Method for
Determining Extreme Pressure Properties of Lubricating Greases Using A High-Frequency, Linear-Oscillation (SRV) Test Machine1 This standard is issued under the ﬁxed designation D 5706; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript superscript epsilon (e) indicates an editorial change since the last revision or reapproval.
1. Scope Scope
coefffıcient ıcient of fricti friction, on, µ or f , n—in tribology tribology, the 3.1.2 coef dimens dimension ionles lesss ratio ratio of the fricti friction on force force ( F ) betw betwee een n two two bodies to the normal force ( N ) pressing these bodies together. G40 3.1.3 Hertzian contact area , n —the apparent area of contact between two nonconforming solid bodies pressed against each other, as calculated from Hertz’ equations of elastic deformaG40 tion. 3.1.4 Hertzian contact pressure magnitude of the pressure , n—the magnitude pressure at any speciﬁed location in a Hertzian contact area, as calculated from Hertz’ equations of elastic deformation. G40 3.1.5 lubricant , n—any material material interpose interposed d between between two surfaces surfaces that reduces reduces the friction friction or wear, or both, between between them. D 4175 3.1.6 lubricating grease , n —a semiﬂuid to solid product of a dispersion of a thickener in a liquid lubricant. D 217 22.214.171.124 Discussion—The dispersion of the thickener forms a two-ph two-phase ase system system and immobi immobiliz lizes es the liquid liquid lubric lubricant ant by surface tension and other physical forces. Other ingredients are commonly included to impart special properties. 3.1.7 thickener , n —in lubricating grease , a substance composed posed of ﬁnely ﬁnely divide divided d solid solid partic particles les disper dispersed sed in a liquid liquid lubricant to form the grease structure. D 217 126.96.36.199 Discussion—The —The thicke thickener ner can be ﬁbers ﬁbers (such (such as various metallic soaps) or plates or spheres (such as certain non-soap thickeners) which are insoluble or, at most, only very slightly soluble in the liquid lubricant. The general requirements are that the solid particles be extremely small, uniformly dispersed, and capable of forming a relatively stable, gel-like structure with the liquid lubricant. 3.1.8 Ra, n—in measurin measuring g surface surface ﬁnish, ﬁnish, the arithmet arithmetic ic average of the absolute distances of all proﬁle points from the mean line for a given distance. 6 3.1.9 Rz (DIN), n —in measuring surface ﬁnish, the average of all Ry values values (peak to valley valley heights) heights) in the assessment assessment 7 length. 3.1.10 Ry, n—in measur measuring ing surfac surfacee ﬁnish, ﬁnish, the vertic vertical al
1.1 This test method method covers covers a procedure procedure for determin determining ing extreme pressure properties of lubricating greases under highfrequency frequency linear-oscil linear-oscillati lation on motion motion using the SRV SRV test machine. This test method can also be used for evaluating extreme pressure properties of lubricating ﬂuid. 1.2 The values values stated in SI units are to be regarded regarded as the standard. The values given in parentheses are for information only. standard rd does not purport purport to addre address ss all of the 1.3 This standa safe safety ty conc concer erns ns,, if any any, asso associ ciat ated ed with with its its use. use. It is the the responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use. 2. Referenced Documents 2.1 ASTM Standards: D 217 217 Test Method Method for Cone Cone Penetr Penetrati ation on of Lubric Lubricati ating ng 2 Grease D 4175 4175 Termino erminolog logy y Relati Relating ng to Petrol Petroleum eum,, Petrol Petroleum eum 3 Products, and Lubricants G 40 Terminology Terminology Relating to Wear and Erosion 4 2.2 Other Standard: Standard: DIN 17230 Roller Roller Bearing Steels Steels 5 3. Terminology 3.1 Deﬁnitions: 3.1.1 break-in, n—in tribology , an initial transition process occurring in newly established wearing contacts, often accompanied by transients in coefficient of friction or wear rate, or both, both, which which are unchar uncharact acteri eristi sticc of the given given tribol tribologi ogical cal G40 system’s long-term behavior.
This This test method method is under under the jurisdicti jurisdiction on of ASTM Committee Committee D-2 on Petroleum Products and Lubricantsand is the direct responsibility of Subcommittee D02.G0.04on Functional Tests Related to Friction, Wear and EP. Current Current edition approved approved June 10, 1997. 1997. Published Published October 1997. 1997. Originally Originally published published as D 5706 – 95. Last previous previous editioin D 5706 – 95. 2 Annual Book of ASTM Standards Standards,, Vol 05.01. 3 Annual Book of ASTM Standards Standards,, Vol 05.02. 4 Annual Book of ASTM Standards Standards,, Vol 03.02. 5 Available from Beuth Verlog Verlog GmbH, Burggrafenst Burggrafenstrasse rasse 6, 1000 Berlin 30, Germany.
6 Amstutz, Hu, “Surface Texture: The Parameters,” Bulletin MI-TP-003-0785, Sheffield Measurement Division, Warner and Swasey, 1985, p. 21. 7 Amstutz, Hu, “Surface Texture: The Parameters,” Bulletin MI-TP-003-0785, Sheffield Measurement Division, Warner and Swasey, 1985, pp. 31, 29.
SRV Test Machine
5. Signiﬁcance and Use
distance between the top of the highest peak and the bottom of the deepest valley in one sampling length. 8 3.2 Deﬁnitions of Terms Speciﬁc to This Standard: 3.2.1 extreme pressure , adj—in lubrication —characterized by metal surfaces in contact under high-stress rubbing conditions. 3.2.2 seizure, n—localized fusion of metal between the rubbing surfaces of the test pieces. 188.8.131.52 Discussion—In this test method, seizure is indicated by a rise in the coefficient of friction, over steady state, of greater than 0.2. In severe cases, a stoppage in the motor will occur. 3.2.3 SRV , n—Schwingung, Reibung, Verschleiss (German); oscillating, friction, wear (English translation).
5.1 This laboratory test method can be used to quickly determine extreme pressure properties of lubricating greases at selected temperatures speciﬁed for use in applications where high-speed vibrational or start-stop motions are present with high Hertzian point contact. This test method has found wide application in qualifying lubricating greases used in constant velocity joints of front-wheel-drive automobiles. Users of this test method should determine whether results correlate with ﬁeld performance or other applications. 6. Apparatus 6.1 SRV Test Machine9, illustrated in Fig. 1 and Fig. 2. 7. Reagents and Materials
4. Summary of Test Method
7.1 Test Balls9, 52100 steel, 60 6 2 Rc hardness, 0.025 6 0.005-µm Ra surface ﬁnish, 10-mm diameter. 7.2 Lower Test Disk 9, 52100 steel, 60 6 2-Rc hardness, 0.45 to 0.65-µm Rz lapped surface, 24-mm diameter by 7.85 mm thick.
4.1 This test method is performed on an SRV test machine using a steel test ball oscillating against a steel test disk with lubricant between them. Test load is increased in 100-N increments until seizure occurs. The load, immediately prior to the load at which seizure occurs, is measured and reported.
NOTE 2—Test pieces made to 100 Crb steel (DIN 17230) are equivalent.
NOTE 1—Test frequency, stroke length, temperature, and ball and disk material can be varied to simulate ﬁeld conditions. The test ball yields point-contact geometry. To obtain line or area contact, test pieces of differing conﬁgurations can be substituted for the test balls.
9 The sole source of supply of the apparatus known to the committee at this time is Optimal Instruments GmbH, Friedenstrasse 10, D-81671 Munich, Germany. If you are aware of alternative suppliers, please provide this information to ASTM Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee,1 which you may attend.
8 Amstutz, Hu, “Surface Texture: The Parameters,” Bulletin MI-TP-003-0785, Sheffield Measurement Division, Warner and Swasey, 1985, p. 25.
9.4 Ensure the machine is unloaded (indicated by a load reading of −13 or −14 N) and carefully place disk containing the lubricating grease specimen and test ball on the test area platform. 9.5 Tighten both the ball and disk clamps until resistance to tightening just begins. Then load unit to 100 N and tighten the ball and disk clamps to a torque of 2.5 N·m. Reduce the load to 50 N for break-in. 9.6 Turn on the heater control and set to the desired temperature. 9.7 Set the load charge ampliﬁer to the setting that corresponds to the 400-N load. 9.8 Change the load charge ampliﬁer at each load in accordance with the manufacturer’s instructions when the coefficient of friction at each test load is to be studied. 9.9 When the temperature has stabilized, turn on the chart recorder and depress the drive start toggle switch until the timer begins to count and then adjust the stroke amplitude knob to 1.00 mm. 9.10 When the digital timer reaches 30 s, increase the load to 100 N using the slow ramp speed rate and maintain this load for 2 min. The 2-min interval includes the loading ramp sequence. Increase the load by 100 N every 2 min using the slow ramp until a load of 1200 N is reached, or the load limit of the test apparatus is attained, or failure occurs. Failure is indicated by a rise in coefficient of friction of greater than 0.2 over steady state or a stoppage in the oscillating of the test machine.
Test Specimen Diagram
7.3 n-Heptane, reagent grade. NOTE 3—Warning: Flammable. Health hazard.
7.4 Isopropanol, reagent grade. NOTE 4—Warning: Flammable. Health hazard.
7.5 Toluene, reagent grade. NOTE 5—Warning: Flammable. Health hazard.
7.6 Cleaning Solvent — a mixture of equal volumes of n-heptane, isopropanol, and toluene. NOTE 6—Warning: Flammable. Health hazard.
8. Preparation of Apparatus
NOTE 8—Because a 30-s break-in at 50 N is used, the load increase times will occur on the half minute of even minutes.
8.1 Turn on the test machine and chart recorder and allow to warm up for 15 min prior to running tests. 8.2 Select the friction data to be presented in the crest peak value position in accordance with the manufacturer’s directions.
9.11 When the 1200-N load run or maximum load of the test apparatus is completed or failure occurs, turn off the heater control, release the load to minimum setting, (typically −13 or −14 N), and remove the test ball, disk, and lubricating grease test specimen.
NOTE 7—In most cases, this is accomplished by positioning the sliding switch on electronic card NO. 291.35.20E (front side of electronics behind the front panel) and the sliding switch located on the back panel of the control unit.
NOTE 9—The SRV test machines available after 1992 have a maximum load of 1400 N.
8.3 Turn the amplitude knob to ZERO. 8.4 Switch the stroke adjustment to AUTO position. 8.5 Set the frequency to 50 Hz. 8.6 Set the desired span and calibrate the chart recorder in accordance with the manufacturer’s instructions. Select the desired chart speed.
10. Report 10.1 Report the following information: 10.1.1 Report all parameters used to evaluate material as follows: 10.1.1.1 Temperature, °C, 10.1.1.2 Stroke, mm, 10.1.1.3 Frequency, Hz, 10.1.1.4 Test ball, 10.1.1.5 Test disk, and 10.1.1.6 Lubricating grease test specimen. 10.2 Report the highest test load at which no seizure occurred.
9. Procedure 9.1 Clean the test ball and disk by wiping the surfaces with laboratory tissue soaked with the cleaning solvent. Repeat wiping until no dark residue appears on the tissue. Immerse the test ball and disk in a beaker of the cleaning solvent under ultrasonic vibration for 10 min. Dry the test ball and disk with a clean tissue to ensure no streaking occurs on the surface. 9.2 Place a small amount (approximately 0.1 to 0.2 g, the size of a pea) of lubricating grease to be tested on the cleaned test disk in an area such that overlapping with previous wear scars will not occur. 9.3 Place the cleaned test ball on the top and in the middle of the lubricating grease specimen so that the lubricating grease makes a circular symmetric pad between the test ball and disk.
11. Precision and Bias 11.1 Eighteen cooperators tested eight greases having average load carrying capacities in the SRV apparatus ranging from approximately 200 N to approximately 700 N. The statistical analysis of data from this interlaboratory test program can be obtained from ASTM Headquarters by requesting Research Report RR:D-2:1410. 3
D 5706 11.2 The following criteria should be used for judging the acceptability of results (95 % probability) for lubricating greases which have load carrying capacities of 1200 N or less in the SRV apparatus. 11.2.1 Repeatability —The difference between successive results obtained by the same operator with the same apparatus under constant operating conditions on identical test material would, in the long run, in the normal and correct operation of the test method exceed the following values only in one case in twenty.
and independent results obtained by different operators working in different laboratories on identical test materials would, in the long run, exceed the following values only in one case twenty. For tests run at 50°C: 1.3 X For tests run at 80°C, 1.2 ~X 1 122!
where: X 5 the average of two results, N. 11.3 Bias—The evaluation of load-carrying capacity of lubricating grease by this test method has no bias because load-carrying capacity can be deﬁned only in terms of the test method.
For tests run at 50°C: 0.7 X For tests run at 80°C: 0.6 ~ X 1 122 !
where: X 5 the average of two results, N.
11.2.2 Reproducibility —The difference between two single
12.1 extreme pressure; lubricating grease; oscillating; SRV
The American Society for Testing and Materials takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, 100 Barr Harbor Drive, West Conshohocken, PA 19428.